**HAL Id: tel-01492946**

**https://tel.archives-ouvertes.fr/tel-01492946**

Submitted on 20 Mar 2017
**HAL is a multi-disciplinary open access**
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**alloys under high pressure**

### Yaroslav Kvashnin

**To cite this version:**

Yaroslav Kvashnin. Ab initio theory of ferromagnetic transition metals and alloys under high pressure. Condensed Matter [cond-mat]. Université de Grenoble, 2013. English. �NNT : 2013GRENY032�. �tel-01492946�

Pour obtenir le grade de

**DOCTEUR DE L’UNIVERSIT ´**

**E DE GRENOBLE**

Sp ´ecialit ´e : **Physique de la Mati `ere Condens ´ee et du Rayonnement**

Arr ˆet ´e minist ´eriel : 7 ao ˆut 2006

Pr ´esent ´ee par

**Yaroslav O. KVASHNIN**

Th `ese dirig ´ee par**Patrick BRUNO**
et codirig ´ee par**Luigi GENOVESE**

pr ´epar ´ee au sein **European Synchrotron Radiation Facility (ESRF)**
et de**l’ ´Ecole Doctorale de Physique**

**Ab initio**

_{study of ferromagnetic}

_{study of ferromagnetic}

**transition metals and alloys under**

**high pressure**

Th `ese soutenue publiquement le**2 Octobre 2013,**
devant le jury compos ´e de :

**Alexander I. LICHTENSTEIN**

Prof., Institute for Theoretical Physics, Hamburg University, Rapporteur

**M ´ebarek ALOUANI**

Prof., Institut de Physique et Chimie des Mat ´eriaux de Strasbourg, Rapporteur

**Josef KUDRNOVSK ´Y**

Dr., Institute of Physics, Prague, Examinateur

**Claudine LACROIX**

D.R. CNRS, Institut N ´eel, Grenoble, Examinateur

**Patrick BRUNO**

Prof., Theory group, ESRF, Grenoble, Directeur de th `ese

**Luigi GENOVESE**

First of all, this thesis would never appear without valuable discussions and support provided by my supervisors Luigi Genovese and Patrick Bruno. Their guidance was of tremendous help and can hardly be overestimated. I also appreciate the amount of freedom which I have been given in terms of the choice of research directions and collaborations.

Raffaella Torchio and Sakura Pascarelli have initiated the project on x-ray dichroism and I was very glad to work in such a team. Nearly all experimental data presented in this manuscript are provided by them.

I thank also Alexei Bossak, Gaston Garbarino and staff of the ID18 for their assistance with the M¨ossbauer experiment. Luckily, none of the ESRF’s equipment went off ! The atmosphere in the Theory group has always been very friendly. The sense of humor of Tim Ziman (Thanks for proofreading) and Andres Cano is something I shall miss. Together with Efim Kats they made each coffee-break a pleasant journey.

I am deeply indebted to Alexander Yaresko for thousands of e-mails which were ex-changed between us and for all the time he dedicated to explain me the physics. Our meetings with Andrei Rogalev were also very fruitful for me.

My stays in Prague were unforgettable. I thank Josef Kudrnovsk´y, Vaclav Drchal, Ilja Turek and Vaclav Janis for the arrangement of these visits and our joint discussions. Working with Pieter Glatzel was a fantastic experience. Those internships at the ID26 have influenced my way of thinking. Thank you for that!

I did my master studies at the Ural Federal University and it is worth thanking the staff of the Department of Theoretical Physics and Applied Mathematics. The background, which I acquired there, was sufficient to perform the Ph.D. and I am grateful to my alma mater and teachers for that. I am much obliged to Vladimir V. Mazurenko for introducing me to the field of band structure modeling and magnetism.

I really appreciate the help and support which was provided by Kristina and Dirk, so I could feel at home in Grenoble. Yann, Theo and Eddy are very inspiring guys - they are part of me. Special thanks to my parents and friends for the words of encouragement.

Acknowledgements i

Abbreviations iv

Abstract vi

Resum´e vii

Introduction 1

1 Computational methods in band structure modeling 5

1.1 Hartree-Fock method. . . 5

1.2 Density Functional Theory . . . 8

1.3 XC Approximations . . . 9

1.4 Realizations of the DFT . . . 11

1.4.1 Muffin-tin orbitals . . . 12

1.4.2 Plane waves . . . 14

1.4.2.1 Pseudopotentials . . . 15

1.4.2.2 Non-linear Core Correction (NLCC) . . . 16

1.4.3 Linearized Augmented Plane Waves (LAPW) . . . 17

1.4.4 Wavelets. . . 17

1.5 Drawbacks of DFT-based methods . . . 20

1.6 Practical applications of the DFT formalism . . . 21

1.6.1 Structural properties . . . 22

1.6.2 Magnetism: Mapping on the Heisenberg model . . . 23

1.6.2.1 Frozen magnons simulations . . . 27

1.7 Conclusions . . . 28

2 K-edge XMCD study of transition metals under high pressure 30 2.1 Introduction: experimental technique . . . 30

2.2 Theoretical interpretation of XMCD spectra . . . 32

2.3 Bulk Ni: an example of persistent ferromagnet . . . 34

2.4 Orbital magnetism in hcp Co under pressure . . . 39

2.4.1 Simple view on the evolution of L and S under pressure . . . 41

2.5 Competing phases in FeCo alloy . . . 42

2.5.1 X-ray experiments . . . 43

2.5.2 Phase diagram from first principles . . . 44 ii

2.6 Conclusions . . . 49

3 High-pressure phase of FePd3 ordered alloy from first principles 51 3.1 Introduction. . . 51

3.2 Modeling of incommensurate magnetic structures . . . 53

3.2.1 Spin spirals . . . 54

3.2.2 Canted spin states . . . 57

3.3 Heisenberg exchange parameters . . . 58

3.4 Extended Heisenberg model . . . 61

3.5 Triple-Q phase . . . 64

3.6 Relation to experiments . . . 66

3.7 Conclusions . . . 67

4 Evaluation of stress in the DFT 69 4.1 Introduction. . . 69

4.2 Stress contributions in the PSP formalism . . . 71

4.3 Tests and comparisons . . . 73

4.3.1 Bulk Si . . . 73

4.3.2 SrTiO3 and LaAlO3 . . . 75

4.4 NLCC and intrinsic stress . . . 77

4.5 NLCC and intrinsic stress: Results . . . 78

4.6 Conclusions . . . 80

Conclusions 82 A General equations for the spin wave energies 85 A.1 Collinear magnets with several sublattices . . . 85

A.2 Noncollinear magnetic structures . . . 88

B Derivation of expressions for stress tensor in the DFT 89 B.1 Kinetic stress . . . 89

B.2 Stress tensor from the Hartree energy . . . 90

B.3 Local part of the PSP . . . 92

B.3.1 Long-range part . . . 92

B.3.2 Short-range part . . . 93

B.4 Non-local part of the PSP . . . 94

B.5 XC contribution . . . 96

B.6 Ion-ion impact . . . 96

DFT Density Functional Theory DOS Density Of States

XMCD X-ray Magnetic Circular Dichroism

WF WaveFunction MF Mean Field HF Hartree-Fock GS Ground State HK Hohenberg-Kohn XC eXhange-Correlation KS Kohn-Sham SC Self-Consistent

L(S)DA Local (Spin) Density Approximation GGA Generalized Gradient Approximation

PW Plane Wave

MT Muffin-Tin

ASA Atomic Sphere Approximation

ES Empty Sphere

LMTO Linear Muffin-Tin Orbital

BC Boundary Condition

FFT Fast Fourier Transform

PSP PSeudoPotential

PAW Projector Augmented Wave NLCC Non-Linear Core Correction

FP Full-Potential

DMFT Dynamical Mean Field Theory iv

OP Orbital Polarization FM FerroMagnetic AFM AntiFerroMagnetic HS High Spin LS Low Spin NM NonMagnetic PM ParaMagnetic FiM FerriMagnetic SW Spin Wave

INS Inelastic Neutron Scattering

BZ Brillouin Zone

R/LCP Right/Left Circular Polarization

DAC Diamond Anvil Cell

SOC Spin-Orbit Coupling

XAS X-ray Absorption Spectroscopy XRD X-Ray Diffraction

PBE Perdew-Burke-Ernzerhof NFS Nuclear Forward Scattering

SS Spin Spiral

FU Formula Unit

DLM Disordered Local Moment

CPA Coherent Potential Approximation

NN Nearest-Neighbor

GTH Goedecker-Tutter-Hartwigsen HGH Hartwigsen-Goedecker-Hutter MIT Metal-Insulator Transition

The subject of the present thesis is the investigation of magnetic properties of transition metals and their alloys under high pressure by means of first-principles calculations. First, the results of the K-edge x-ray magnetic circular dichroism (XMCD) experiments on Ni and Co are interpreted. It is shown that the experimental pressure evolution of the data should be compared with that of the p-projected orbital magnetization. I emphasize that the spin and orbital moments have different behavior upon compression. In the case of FeCo alloy the structural transition occurs under the pressure of 35 GPa. I propose that the emergence of antiferromagnetism can explain the disappearance of the XMCD signal at the Fe and Co K-edges.

Then, the phase transformation in FePd3, induced under pressure of 12 GPa, is inves-tigated. I demonstrate that the system is described by an extended Heisenberg model, containing strong biquadratic exchange interactions. According to the results, FePd3 undergoes a transition from the ferromagnetic to the noncollinear triple-Q state when compressed.

Finally, the implementation of the stress tensor in the BigDFT software package is pre-sented. It is shown that an explicit treatment of core electrons can considerably reduce the errors introduced by the pseudopotentials. Thus the estimates of the structural properties can be improved.

Le sujet de cette th`ese porte sur l’´etude des propri´et´es magn´etiques de m´etaux de tran-sition et leurs alliages sous haute pression au moyen de calculs ab initio.

D’abord, les r´esultats de mesures de dichro¨ısme magn´etique circulaire des rayons X (XMCD) au seuil K du nickel et du cobalt sont interpr´et´es. Je montre que les donn´ees exp´erimentales doivent ˆetre compar´ees `a celle de l’aimantation d’orbite projet´ee sur les ´etats p. Je mets en avant que la pression affecte diff´eremment le spin et le moment orbitalaire.

Dans le cas de l’alliage FeCo, la transition structurelle s’effectue sous une pression ap-pliqu´ee de l’ordre de 35 GPa. Je propose que l’´emergence de l’antiferromagn´etisme peut expliquer la disparition du signal XMCD au seuil K du fer et du cobalt.

Ensuite, la transformation de phase dans FePd3, induite sous une pression de 12 GPa, est ´etudi´ee. Je d´emontre que le syst`eme est d´ecrit par un mod`ele de Heisenberg ´etendu, contenant interactions d’´echange biquadratiques forts. Selon nos r´esultats, FePd3 subit une transition de l’etat ferromagn´etique ´a l’´etat triple-Q non-colin´eaire, lorsqu’il est compress´e.

Enfin, une mise en oeuvre du tenseur des contraintes dans le code BigDFT est pr´esent´ee. Il est montr´e qu’un traitement explicite des ´electrons de coeur permet de r´eduire con-sid´erablement les erreurs introduites par les pseudo-potentiels. Ainsi, les estimations des propri´et´es structurales peuvent ˆetre am´elior´ees.

Understanding the processes deep inside the Earth has been a dream of humanity since antiquity. There are lots of mysteries, as, for example, the origin of our planet’s magnetic field. This problem is still under debate – a few models have been proposed but none of them is able to give an unequivocal answer.

Unfortunately, the level of today’s technology allows us to dig holes no deeper than a few kilometers. So there is still a very long way to the Earth’s core. Nonetheless, we know the constitution of the mantle and more deeper regions of the Earth. There are such elements as oxygen, magnesium, silicon and iron. The inner core of our planet is made predominantly of iron and nickel. These transition metal elements are of the greatest interest, since at normal conditions they possess spontaneous magnetization. We can also estimate the most important thermodynamic parameters in this region: pressure in the inner core region should be about 300 GPa and temperature exceeds 4000 K1. Thanks to the use of diamond anvil cells it has become possible to reach pressures of the order of 100 GPa. Regarding the second parameter, today’s lasers are able to heat the matter up to the necessary level. So, in principle, the Earth’s core conditions can be reconstructed in a modern laboratory. In combination with element-selective techniques like x-ray spectroscopy, this becomes a powerful tool for the investigation of the electronic and magnetic properties of the Earth’s interior.

Moreover, from a fundamental point of view an application of pressure to the transition metals allows us to verify existing models of magnetism. The reality is that there is no unified theory which could a priori describe any magnet. Hence, in studying a particular system one is forced remain in one of two frameworks, depending on the

1

In spite of such high temperatures, the inner core is solid, since the tremendous pressure pushes the melting point of iron-nickel alloys much higher.

**P**

### E

### E

### N

### (E

### )

*i*

*f*

### E

FFigure 1: _{Schematic representation of densities of states (N (E)) in ferromagnetic}
system and its changes upon application of pressure. Bands become wider due to

increase of orbital overlap, while magnetic splitting tends to decrease (∆i> ∆f). degree of localization of the magnetization density. Magnetic systems which consist of relatively well-localized spins (in real space) are usually studied within a Heisenberg model. On the contrary, itinerant magnets, characterized by delocalized magnetization density, are treated with the help of Stoner model [156].

The magnetism in transition metals arises from the unfilled 3d electron shell. The spatial distribution of 3d WFs is such that electrons are located right on the border between atomic localization and formation of wide electronic bands (see e.g. Ref. [155][p. 223]). As a result, the very same 3d states can exhibit opposite behavior depending on their environment and filling. Thus compression, i.e. a change of interatomic distances, allows one to adjust the localization in a precisely controlled way.

Effects of pressure on electronic structure of ferromagnetic metals are known. The most general trends are shown on Fig. 1. As the interatomic distance decreases, the overlap between electrons wavefunctions gets larger, which leads to their delocalization. Ac-cording to Stoner theory, the density of states at the Fermi level (DOS(Ef)) should exceed a certain threshold in order to favour appearance of ferromagnetic order. There-fore it is reasonable to assume that application of pressure should eventually lead to the disappearance of magnetism.

This suggested tendency is indeed observed in experiments, but such a magnetic tran-sition does not really occur for 3d metals. Structural trantran-sitions usually take place at lower pressures than needed to violate the Stoner criterion. For instance, such situation appears in bcc iron, which undergoes a transition to a non-magnetic hcp phase [115].

In the present thesis we will try to get deeper insight into the change of magnetic properties of 3d systems with the help of the Heisenberg Hamiltonian. The key quantity of the present theory is the set of interatomic exchange parameters Jij. These parameters will be extracted from realistic band structure calculation for a particular system and their pressure dependence will be studied. Their change with lattice contraction is not straightforward to predict. On one hand, reduction of the lattice constant leads to increase of the overlap. Therefore the so-called direct exchange interaction should become larger. On the other hand, the local magnetic splitting gets smaller, as was already shown. Thus there are two general tendencies which compete with each other. The problem gets more complicated due to the fact that in metallic systems the J’s are rather long-ranged in space. It turns out that magnetic moments separated by several Angstr¨oms are still coupled, and this coupling is not related to direct overlap of the orbitals. Hence, this requires the use of electronic structure calculations which are able to provide a detailed description of electronic bands.

### Organization of the thesis

The thesis is organized as follows:

Chapter 1 contains an overview of ab initio band structure methods. It is primarily devoted to the Density Functional Theory (DFT), which is the main instrument in the present study. Drawbacks and merits of different realizations of this theory are discussed. Special attention is given to the study of structural and magnetic properties. Such quantities as stress, pressure and magnetic couplings are formulated in terms of the present apparatus.

Chapter2 concerns analysis of K-edge x-ray magnetic circular dichroism (XMCD) data in various 3d systems. First, a historical overview is given of present experimental technique, as well as its theoretical modeling. Next, XMCD spectra measured on bulk Ni, Co and FeCo alloys are analyzed with the help of first-principles calculations. In Chapter3an analysis of magnetic interactions in FePd3 is presented. Based on these results, a new magnetic ground state is suggested to be stabilized under pressure in this system. Various experiments which could confirm these findings are proposed.

Chapter 4 is devoted to calculation of the stress tensor within a particular DFT code. The computational scheme is applied to various classes of materials and the results are compared with prior realizations of this formalism. Further, an emphasis is given to the impact of core electrons on structural properties of quantum systems. The importance of this contribution is discussed.

## Computational methods in band

## structure modeling

The so-called ab initio (i.e. first-principles) methods for electronic structure calculations are widely used in modern science. They allow us to simulate and sometimes even predict properties of the actual materials with no use of any adjustable parameters. These methods require almost no information about the system: it is just necessary to know its crystal structure in order to start the calculation. Then any observable quantity, like equilibrium volume, magnetization, ionic charge and others can be extracted from the calculation and sometimes directly compared with experimental data. The range of application of these methods spreads from the material science, solid state physics, chemistry and biology. This is how science is made nowadays, but such progress was achieved only recently. Therefore, before describing the state-of-the-art methods this chapter will start by the historical overview of the electronic structure modelling.

### 1.1

### Hartree-Fock method

To have such powerful approaches, able to deal with the quantum systems consisting of many particles, was one of the biggest challenges for physics of XX’th century. One of the first methods was proposed by Hartree in 1928 [76]. At that time it was already known that the properties of quantum systems are governed by the Schr¨odinger equa-tion. In particular, a system which consists of N atoms and n electrons coupled via

electromagnetic interaction is described by the following Hamiltonian:
ˆ
H =_{−}1
2
n
X
i=1
∇2ri+
1
2
X
i6=j
1
| ~ri− ~rj |−
N
X
I=1
n
X
i=1
ZI
| ~RI − ~ri|
−
N
X
I=1
1
2MI∇
2
RI +
1
2
X
I6=J
ZIZJ
| ~RI − ~RJ |
,
(1.1)

where ~ri and ~RI are the positions of electrons and atoms, respectively. Letters Z and M denote charge and mass of each nucleus. This equation is written in the atomic units: mass is in the units of electron mass me and charge is measured in electronic charge | e |. We are eventually interested in finding the eigenvalues and eigenvectors of the corresponding operator, which will give an access to all observable properties. But the Hilbert space dimension is 3(N + n), which makes it certainly impossible to diagonalize the matrix explicitly.

Nonetheless, the last two terms in the right-hand side (r.h.s.) of Eq. (1.1) describe the dynamics of ions, which are at least ≈1836 times heavier than electrons. Therefore, it is well justified to decouple these degrees of freedom from electronic ones. This can be done using so-called Born-Oppenheimer approximation [17], which consists in treating the ions classically. It is assumed that the ionic positions are completely frozen and they form an electrostatic potential which acts on electrons. Hence the atomic positions and charges enter the Eq. (1.1) as the external parameters in our quantum problem.

This way the dimension of the problem is reduced (to 3n variables) and is associated with electronic degrees of freedom solely. However, the Hilbert space dimension is still too large for the real compounds.

Therefore we are forced to use approximations in order to simplify the initial problem. The idea of Hartree was to map the many-body problem into a non-interacting parti-cle problem in an effective potential. Hence, each electron is moving in some central field created by nucleus and other electrons. Within the proposed method the many-electron wavefunction (WF) Ψ(r1, r2, ..., rn) is represented as a product of one-particle wavefunctions:

each of those satisfies the one-particle Shr¨odinger equation: h

−1_{2}∇2+ Vext+ Φi
i

ψi(ri) = εiψi(ri), (1.3)

where Vext is external lattice potential and Φi is a potential of electron-electron inter-action. So the influence of all other electrons on a certain particle is taken into account in a mean-field (MF) manner and enters the Hamiltonian via the terms of the following type:

Uij = ZZ

d~r1d~r2 | ψi( ~r1)|2Vee(~r1− ~r2)| ψj( ~r2)|2, (1.4)

where Uij is a direct Coulomb interaction between wavefunctions corresponding to the states i and j. It has the form of interaction between two charge densities like in classical electrodynamics. This was a so-called Hartree approximation.

Later it was shown that during the construction of a many-body WF it is necessary to satisfy rules of Fermi statistics: i.e. the antisymmetry of fermionic operators with respect to the swap of two particles [53]. The r.h.s. of Eq. (1.2) becomes a determinant of different ψ’s, called “Slater determinant” [151], namely:

Ψ(r1, r2, ..., rn) = ψ1(r1) ψ1(r2) . . . ψ1(rn) ψ2(r1) ψ2(r2) . . . ψ2(rn) . . . . ψn(r1) ψn(r2) . . . ψn(rn) . (1.5)

This is the base of the Hartree-Fock technique. Reformulation of Ψ(r1, r2, ..., rn) has an important consequences and results in the appearance of additional contributions to Φi - the non-local exchange terms of the following type:

Jij = ZZ

d~r1d~r2ψi∗( ~r1)ψ∗j( ~r2)Vee(~r1− ~r2)ψj( ~r1)ψi( ~r2). (1.6)

It is worth emphasizing that this is a purely quantum effect, which originates from Pauli exclusion principle. However, exchange term is an essential quantity in the theory of magnetism1. So the quantity Jij is important in the present context and will be widely

1

It is fascinating to realize that we have actual magnetic materials solely thanks to laws of quantum mechanics.

used throughout this thesis.

Concerning the Hartree-Fock method, it is worth noting, that in some cases the system’s WF should be described via a linear combination of Slater determinants, corresponding to the states with similar energies. In principle, this procedure gives a reasonably exact wavefunction, but the computational effort grows very fast with increase of the number of particles. Hence, in practice, the method is only used if the quantum problem is (or can be reduced to) relatively small.

### 1.2

### Density Functional Theory

Due to the above-mentioned reasons, it is clear the use of WFs is not so efficient for
realistic systems. A big step forward in the problem of finding ground state (GS) energy
was made by Hohenberg and Kohn in 1964 [78,96]. They suggested to operate with
elec-tronic density (ρ) instead. Their celebrated Hohenberg-Kohn (HK) theorem states that
for a given n particles the GS charge density determines uniquely the external potential
of the electronic Hamiltonian. In the other words, there is a one-to-one correspondence
between GS density and external potential, which controls the inhomogeneity of the
electron gas. The total energy (E) is a functional of ρ and reaches its minimum for true
GS density ρ0:
E[ρ] = T0[ρ] +
Z
d~rρ(~r)Vext(~r) +
1
2
ZZ
d~rd~r′ρ(~r)ρ(~r′)
| ~r − ~r′ _{|} + Exc[ρ], (1.7)
where T0 is the kinetic energy contribution and Exc is the exchange-correlation (XC)
term. The second and third terms are ion Coulomb interaction and
electron-electron interactions, respectively. The latter contribution has exactly the same form as
in Hartree method and therefore is called Hartree potential. Instead of Fock
contribu-tions, one introduces the Exc term which is called to mimic the exchange part and also
many-body (correlation) effects. We can define a new quantity ǫxc(~r) – the so-called XC
density per particle which will be associated with Exc, so that:

Exc[ρ] = Z

DFT would be an exact theory if we knew the true form of this term, which is missing. Hence it is inevitable to use some approximations to Excand their choice plays a crucial role in the theory. This problem will be addressed later in more details.

Having defined a suitable XC term, the GS of the system can be obtained. We can use an advantage of the DFT that it is not important from which WFs the electron density is built. Therefore for practical applications ρ can be defined as:

ρ(~r) = n X i=1

|ψi(~r)|2, (1.9)

where n is a number of electrons (which is fixed). Varying the Eq. (1.7) with respect to new variables ψi(~r) with an additional constraint for their normalization leads to the system of coupled Kohn-Sham (KS) equations:

h
−∇2−X
I
2ZI
| ~r − ~RI |
+ 2
Z _{ρ(~}_{r}_{′}_{)}
| ~r − ~r′ _{|}d~r
′_{+ V}
xc(~r)
i
ψi = εiψi, (1.10)

where εi are the Lagrange multipliers that form the spectrum of single-particle states; The XC potential is a functional derivative of Exc, i.e.:

Vxc=

δExc[ρ] δρ(~r) =

d

dρ(ρǫxc[ρ]). (1.11)

System of Eq. (1.10) has to be solved iteratively. One can start calculation with trial WFs, for example a set of isolated ionic states, and solve the Poisson equation to find Hartree potential. Then one has to diagonalize the KS Hamiltonian and construct the new electronic density. The procedure has to be repeated until one reaches the minimum of the total energy E[ρ0]. This is the basic representation of a self-consistent (SC) loop. In practice, there are different strategies for updating the density and several possible choices of the convergence criteria, but we shall omit these details at this stage.

### 1.3

### XC Approximations

As it has already been mentioned, the biggest problem of the DFT is the lack of an exact form of the XC term. There is no universal approximation which could correctly

describe properties of any material. However, for wide range of systems the so-called Local Density approximation (LDA) is rather successful.

In the present framework the XC density is taken in the form for homogeneous interacting electron gas (h.g.) of the density ˜n, but at each point in space ˜n is substituted for an actual density ρ. Hence ǫxc[ρ] = ǫh.g.xc (ρ(~r)) and one can write explicitly:

Exc[ρ] = Z

ρ(~r)ǫxc(ρ(~r))d~r. (1.12)

Spin-polarized version of LDA, called local spin density approximation (LSDA), is used for magnetic systems. This method introduces two separate densities of electrons with positive and negative spin projections on quantization axis, ρ↑ and ρ↓, respectively. The quantity ǫxc can be parametrized using results of numerical calculations and several realizations are present nowadays [134,167,168].

L(S)DA was implemented in the first realizations of the DFT and immediately showed an impressive performance. Such a simple approximation led to a rather good prediction of band structures of the whole class of conventional semiconductors, alkali and transition metals [88]. In principle, LDA provides the most accurate results for systems, whose electronic density varies rather slowly in space.

The next generation of the XC functionals was built using not only the electronic density but also its gradient, i.e. :

ǫxc(~r) = ǫxc(ρ(~r),|~∇ρ|(~r)). (1.13)

In this case, XC potential, according to Eq. (1.11), is given by:

Vxc(~r) =
d
dρ(ρǫxc[ρ]) +
Z
d~r′_{ρ(~}_{r}′_{)} ∂ǫxc
∂|∇ρ|
δ_{|∇ρ|(~r}′_{)}
δρ(~r) . (1.14)

The first term in the current expression is the same as in the case of the LDA, while the second one represents an additional correction. The present approach is called Generalized Gradient Approximation (GGA) [135].

In most cases, L(S)DA and GGA provide with very similar ground states. GGA often provides better estimates of structure-related quantities, like bulk moduli (B) and equi-librium volume (Ω0) [73]. In terms of other properties, magnetic for instance, usually there are no significant differences between results provided by these two methods. However, these results are not general and there is no a priori knowledge about the choice of the XC approximation for a particular system. A well-known example is elementary iron: LDA predicts its paramagnetic fcc phase to be more stable than ferromagnetic bcc one, which is a real GS of iron in nature, while GGA is able to overcome these unphysical outcomes [176]. On the other hand, GGA faces problems in predicting correctly the stable crystal structure of Fe3Al alloy [104].

In general, GGA shares the same problems with LDA in modeling a certain class of materials, so-called “strongly correlated” systems. This problem will be addressed in the next section.

It’s worth mentioning that these days the list of available functionals is not limited to LDA/GGA types only. An improvement of XC potentials is a stand-alone field of research which develops very fast. For instance, there are attempts to add a fraction of the exact exchange energy, i.e. provide a combination of the DFT with HF methods [12]. The results for some molecular systems have proven that these “Hybrid” functionals provide a more accurate bond length and ionization energy estimations as compared with experimental data [11].

For deeper insight into the constellation of existing functionals the reader is referred to Ref. [113] and references therein. Present study concerns the investigation of magnetic properties of pure transition metals and their alloys. For this type of systems classical LDA/GGA-type functionals are known to be suitable (see e.g. [8]) and will be used throughout this thesis work.

### 1.4

### Realizations of the DFT

In last decades plenty of DFT-based codes have appeared, in spite of the fact that they all implement the same theory. The main reason for these developments is related with an increase of accuracy and ability to treat bigger systems on a reasonable time-scale.

Moreover, certain physical quantities can be accessed more easily depending on the employed formalism.

Different realizations of the DFT can be characterized according to the basis functions
used for expressing the KS orbitals. These basis sets can be divided in two major groups:
the ones which are more localized in reciprocal space (plane waves [PW], for example)
and in direct one (like Gaussian-type orbitals [GTO]2_{).}

As a limiting case one can think of a completely isolated (non-periodic) molecular sys-tem. Clearly, the WFs are difficult to treat using PWs, since they contain too many components in the expansion. Atomic-like functions would be more efficient for this study.

Therefore, before starting the band structure simulation of a certain compound, it is reasonable to inquire whether the system is mainly characterized by highly mobile (de-localized) electrons, which is a typical situation in metals, or it is an insulator with quite localized WFs. Indeed, periodic systems are more difficult to sort: they sometimes exhibit a mixed behavior, but normally can be attributed to one of two groups. Thus an appropriate set of basis functions can be chosen. In other words, the most efficient way is to choose the basis set according to particular needs.

It is sometimes necessary to work with several realizations of the DFT and balance between them. Here we wish to make an overview of several basis sets, each of whose will be used in the present work. Note that the list is not exhaustive, but represents a diversity of the DFT codes. Interested reader is referred to the book by R. Martin [114].

1.4.1 Muffin-tin orbitals

At the time of the first developments of the DFT codes the computers performance was much lower than today. The codes which were written 40 years ago aimed to reduce the computational effort, so the state-of-the-art machines were capable to solve the prob-lem. Thus the first realizations of the DFT contained some additional approximations (beyond intrinsic), which in principle can be avoided nowadays thanks to the progress

2

These functions are widely used in the field of quantum chemistry for studying molecular compounds. Minor attention is paid to this topic in the present thesis, since it is primarily concerns metallic systems.

of computational technology. However, the methods developed at whose times are still used and there are reason for that.

One of the first approaches which incorporated the DFT was similar to the tight-binding method. In this spirit WF of each electron, which is a solution of KS equation (Eq. (1.10)), is approximated as a sum of atomic-like orbitals, centered on a certain atom. Due to the symmetry of the Hamiltonian under consideration, it is reasonable to define a sphere of a certain radius (RM T) around each atom and assign it to this ion. O.K. Andersen [4] suggested to extend these regions so that the entire system will be represented by a sum of overlapping spheres. This way of the space partitioning is called called the atomic sphere approximation [ASA]. For not-so-close-packed crystal structures we can fill the interstitial space with the empty spheres (ES), possessing zeroth charge. At this stage we can make an approximation to the potential and require it to be spherically symmetric inside each sphere and constant outside, so that:

V (~r) =
V (|~r|), if|~r| ≤ RM T
C, if_{|~r| > R}M T
(1.15)

A potential defined this way is called the muffin-tin (MT) one. Inside the sphere our problem is reduced to the Shr¨odinger equation with spherical potential, which solution is known. Core electrons in each ion form localized levels with practically no dispersion which are relatively easy to calculate. Valence electrons that participate in formation of bands, certainly require a more thorough treatment.

Outside of each sphere there is the Laplace equation which has to be solved: _{∇}2Φi = 0.
Hence a true valence WF has to match the boundary conditions (BCs) on the spheres.
Therefore it becomes not only a function of position, but also that of energy.

Andersen’s idea was to linearize this energy-dependence [4], i.e. take first two terms in corresponding Taylor expansion :

ψi(~r) = X lm Almφl(~r, Eν) + Blm ∂φl ∂E(~r, Eν) Ylm(~r), (1.16)

where the sum is over angular momentum quantum numbers (l), φl is a solution of the radial Shr¨odinger equation for the energy Eν inside a MT sphere; and Ylm are Legendre polynomials. Coefficients Alm and Blm are fitted in order to fulfill the BCs.

The linearization energy Eν is usually chosen to be in the center of the corresponding band. Thanks to such choice, the errors due to linearization are efficiently canceled. On the first sight, this looks as a rather crude approximation of the real band structure. In reality this approach was a real breakthrough. It turned out to be quite accurate for real applications and quickly became an essential tool of computational solid state physics.

Why is this method still used ? Its main advantage, especially nowadays, is perfor-mance. A band structure of simple metal can be calculated in few seconds. Use of the ASA is not always physically motivated, but on the other hand it allows to access the local quantities (via occupation matrices) straightforwardly. Since entire space is parti-tioned, one can immediately obtain the magnetization per atom, ionic charge and other important properties. Additionally, an analogy with the tight-binding method makes interpretation of the results quite simple and intuitive.

1.4.2 Plane waves

In one of the most wide-spread realizations of the DFT, the KS wavefunction is repre-sented as a linear combination of orthogonal plane waves:

ψl(~r) = X | ~G|<Gmax

C_{G}l exp i ~G_{· ~r}, (1.17)

where ~G is a vector of reciprocal space. In principle there is only one parameter which has to be adjusted– the energy cut-off which sets the maximal modulus of reciprocal vectors Gmax used in Eq. (1.17). The cut-off is a variational parameter, namely its increase results strictly in lowering the absolute value of the total energy. Hence the accuracy is straightforward to control.

In general this basis set is very convenient to operate with. For instance, in Fourier space
the kinetic part of the Hamiltonian is just diagonal. In addition, these codes widely use
the Fast Fourier Transform (FFT), which gives an almost linear (_{∼ n log n) scaling of}
computational time with respect to number of electrons.

On the other hand, wavefunctions have to be re-orthonormalized on each iteration and this step is the most demanding in the whole SC process. As a result, the overall

computational cost grows as n3 and limits the domain of application of PW’s up to the systems containing few hundred atoms. Nonetheless, PWs is a suitable basis set for periodic and highly-symmetric systems.

1.4.2.1 Pseudopotentials

In practice, the KS WFs strongly oscillate in the vicinity of atomic core. In order to represent such function in Fourier space one will need to drastically increase the size of PW set to obtain reasonable accuracy. This is not efficient and sometimes not even feasible. However, the nucleus charge is largely screened by core electrons. Thus valence electrons – the ones which we are primarily interested in – do not “feel” this bare charge. So the total ionic (i.e. combined nucleus and core electrons) potential can be substituted by another operator, called “pseudopotential” (PSP), which mimics true potential in some region of space. Usually this region is located outside of the sphere of a certain radius (Rcore).

Pseudopotentials are meant to provide a detailed representation of ionic charge influence
on valence electrons. They normally consist of two terms: local and non-local ones. The
first part is a function, which depends solely on the distance from the nucleus, being
purely isotropic. However, in general case, core electrons occupy orbitals with different l
quantum numbers. This brings some anisotropy on the produced potential. In the PSP
present effect is taken into account via an introduction of l_{−dependent terms, called}
“non-local” ones. Thanks to these terms, valence states, characterized by different
l-numbers, are affected differently by core electrons.

With the help of the PSP, the dimension of the problem is reduced (only valence electrons are considered) and size of the basis set is decreased. Although it is highly beneficial, the method has certain drawbacks.

First of all, core electrons do not enter the simulation explicitly and their action is not updated during the SF loop. This is usually not a problem if the system is next to equilibrium volume. However, can cause some undesired effects if one wants to study

properties at ultra-high pressures. As a solution one has to use “harder” PSPs (which
require higher cut-off) with semi-core states treated explicitly3_{.}

Secondly, the construction of the pseudopotential is a procedure, which is rather complex and not easy to automatize. In most cases, users of the PW codes have to use PSPs provided by developers within the same package. In practice, it turns out that a certain PSP represents some physical properties better than others in comparison with all-electron calculations taken as reference. This is not related with the accuracy of the DFT formalism itself and is just due to self-introduced computational errors.

Hence, the construction of a PSP has to be done with care and special attention must be paid to its transferability, i.e. the ability to reproduce well the all-electron behavior of a given atom independently of its chemical environment.

1.4.2.2 Non-linear Core Correction (NLCC)

One of the possibilities to improve the quality of PSPs is inclusion of nonlinear core corrections (NLCC) [108], where the core charge density (ρc) is explicitly introduced. Yet, it is considered to be independent of chemical environment and is frozen during the self-consistent process. Usually, for simplicity, the distribution of the core electrons is represented in a simple analytical form.

In order to understand the importance of such treatment of ρc, it is useful to
con-sider the overall spin polarization of a system, i.e. the following quantity: ξ(~r) =
(ρ↑(~r)− ρ↓(~r)) / (ρ↑(~r) + ρ↓(~r)), where {↑, ↓} denote spin projections. Clearly, ξ is
poorly represented, if core electrons are neglected. In most cases the primary
con-tribution to the total charge density comes from low-lying levels. Even though the spin
density is negligible in the core region, accounting for ρ_{c↑(↓)} affects ξ dramatically. Let
us imagine, for instance, an ionic configuration where all valence electrons have the same
spin projection, e.g. _{|↑↑↑↑↑i . If only valence electrons are considered, then: ξ → 1. }
Tak-ing into account core electrons (suppose that Z >> 1) results into: ξ_{→ 0. Since ξ is an}
important quantity, the NLCC is expected to improve the description of spin-polarized
valence states.

3

This is especially important in the case of Projector Augmented Wave (PAW)[15] formalism. Here the “core ” sphere radius is much larger comparing with classical PSP, so even moderate pressure can cause an overlap of these regions which is, strictly speaking, forbidden.

1.4.3 Linearized Augmented Plane Waves (LAPW)

Present approach is a sort of combination of the methods described above. Here, MT spheres are also introduced, but in a different manner: they do not overlap, leaving the interstitial space untouched.

Within MT sphere the potential is not assumed to be isotropic (_{∼ Y}00), but also contains
higher-order expansion coefficients, so that :

V (~r) = P lm Vlm(~r)· Ylm(~r), if|~r| ≤ RM T P ~ G VG· exp i ~G ~R , if|~r| > RM T (1.18)

Since there is no approximation to the shape of the potential, this method is called “full-potential” (FP). Core levels are re-calculated at each iteration and corresponding contribution to the potential is updated. This is a dramatic difference with respect to previously mentioned techniques. In fact, it allows also to access such nuclear quantities as isomer shifts, hyperfine fields and electric field gradients.

Concerning the WF of valence electrons, it has the same form as given by Eq. (1.16) inside the MT sphere. Outside of this region the WF shows a delocalized character and is expanded in PWs (Eq. (1.17)). Such division results into a very efficient flexibility in the WF representation.

The FP-LAPW method is considered to provide the most precise modeling of the band structure. Usually the results of calculations produced with this technique are used as a reference for comparison with other DFT realizations. The price to pay is compu-tational time: since there are less approximations, the method is more demanding. In addition, access to local quantities is not always straightforward. Projections on atoms are performed within MT spheres, so the interstitial charge density is not attributed to any site. Hence, an attention has to be payed to the choice of RM T.

1.4.4 Wavelets

Wavelets is a special type of functions which was introduced in order to analyze fre-quency components of data. Their name already implies that wavelets must look like local perturbations which starts at some point, oscillates with finite amplitude and then

-4 -2 0 2 4 6 -1

0 1

*x*

Figure 1.1: _{Daubechies wavelet functions of order 2 (red line) and 8 (blue dashed}
line).

attenuates back to zero. Indeed, the shape of these functions reminds particle wave packets from the course of quantum mechanics.

All families are characterized by two fundamental functions in wavelet theory, which are the scaling function φ(x) and the wavelet ψ(x)4.

Fig. 1.1 shows the 2-nd and 8-th order wavelets from the Daubechies family [31]. It is clearly seen that the support length (i.e. an interval where functions are nonzero) widens as the order of wavelets increases. The most important property of wavelet families is that their degrees are in relation. Namely, the functions φ(x) and ψ(x) are defined in such a way that they obey so-called refinement relations:

φ(x) =√2 Pm j=1−m hjφ(2x− j) ψ(x) =√2 m P j=1−m gjφ(2x− j), (1.19)

where hj and gj are the elements of a filter that characterizes the wavelet family, and
m is the order of the wavelet family. In fact, there is no analytical expression for
wavelets, but components of these filter coefficients can be computed exactly, so they are
tabulated. Depending on the form of_{{h}j} and {gj}, wavelets can be be either orthogonal,
biorthogonal or semiorthogonal. In orthogonal wavelets families the following relations

4

between filter coefficients take place: gj = (−1)jh−j+1, P l hl−2ihl−2j = δij, P l gl−2igl−2j = δij, P l gl−2ihl−2j = 0. (1.20)

Eq. (1.19) together with (1.20) establishes correspondence between the scaling functions on a discretized grid of spacing h and another one of spacing h/2. All wavelets properties can be obtained from these expressions. The entire basis set can be built from all possible translations of the mother function centered at the origin by a certain grid spacing h. The mother function is localized and has relatively compact support.

As we have seen, wavelets form a smooth basis set that is localized in both direct and reciprocal space. Thanks to these unique properties, they are of great potential applica-tions. Wavelets have recently became a useful tool for solving differential equations [61]. Since such type of mathematical problems appears almost everywhere, wavelets enter more and more fields of nowadays research.

Just a few years ago an efficient method for solving Poisson equation in different BCs, based on the wavelet-like functions, was suggested[57, 58]. Soon after wavelets were already applied to realistic band structure caculations. Daubechies family as a basis set are incorporated with the PSP formalism and realised in the BigDFT code [59], which will be used in the present thesis.

The primary merit of this approach is an ability to treat systems with different BCs on equal footing. For example, in case of surface BCs one direction, say y, is isolated while two others are periodic. In majority of the DFT codes the modeling of such system would require an enlargement of the unit cell in y-direction, preserving its peri-odicity. Thus the system becomes well-separated from its y-translated replica. But the simulation box has to be extremely large to ensure the cancellation of the long-ranged Coulomb interactions. Hence, an explicit treatment of mixed BCs becomes very ad-vantageous from computational viewpoint. Moreover, charged systems can be treated without introduction of an artificial compensating background, as done, for example, in Ref. [111].

In addition, the code is young, massively parallelized and shows fair performance on nowadays computers [60].

### 1.5

### Drawbacks of DFT-based methods

In previous section a brief overview of several realizations of the DFT was made. Some of them are more accurate than the others due to the presence of approximations to the ionic potential.

However all codes share the same drawbacks which arise from the basic DFT formalism. For instance, there is an intrinsic problem of self-interactions. Since all electrons con-tribute to the Hartree term, it leads to the unphysical consequence that each electron is affected by the field which is partially produced by itself.

Another shortcoming of this technique is that it provides only with the GS at zero tem-perature (T = 0). But in reality we have to deal with materials at finite temtem-perature, thus the lowest state gets mixed with excited ones, like in Boltzmann’s ansatz. Unfor-tunately, there is no direct access to excited states in the present framework. Moreover, the information about higher-lying states is essential, since most often in an experiment the system under consideration is subjected to some perturbation and gets excited from its GS. Post-DFT approaches like time-dependent DFT (TD-DFT)[143] and the GW method[80] were suggested in order to overcome this problem. They are on the level of development.

A serious problem of the DFT is the lack of the many-body (correlation) effects. In the present approach the electrons experience the same average potential which depends on total electron density solely. The corresponding Hamiltonian can be diagonalized resulting in a set of independent particles moving in some MF. In the context of the Hubbard model[79], it means that only the band term (containing hopping) is present. The four-particle (i.e. coupling) term which is responsible for the multiplet structure formation and atomic-like behavior is completely omitted within the DFT formalism. For strongly correlated systems these effects dramatically affect the band structure and therefore the DFT can not provide an accurate model for them. This is exactly the case, for instance, in transition metal oxides and unconventional superconductors like cuprates

and pnictides. Nowadays there are several techniques exist, able to go beyond conven-tional DFT and include some part of correlation effects. Among such approaches the most widely-used are LDA+U [5] method and a conjunction of the DFT and Dynamical Mean Field Theory (DFT+DMFT) [97].

There is another drawback of the conventional DFT which is important for magnetic systems. It is the well-known problem of underestimation of orbital magnetism [26,

28]. There are at least two ways to improve these assessments: the already mentioned LDA+U and the orbital polarization (OP) [20,44,45] techniques. The first one, taking into account part of local correlations, essentially leads to electron localization, which usually results into an augmentation of local quantities like spin and orbital moments. Within second approach an additional term to the Hamiltonian, which reflects the second Hund’s rule, is introduced. Both methods require some ad hoc parameters, even though the possibilities of ab initio determination of them were proposed [45,70].

In the context of the present work it was already mentioned that the DFT provide quite detailed description of transition metals band structures. However, the drawbacks have to be kept in mind while using this technique to study new classes of materials, where a priori knowledge is missing.

### 1.6

### Practical applications of the DFT formalism

Using the DFT it is possible to simulate vast amount of physical and chemical properties of the matter. The aim of the present work does not imply to cover the whole spectrum of its applications, so we will restrict ourselves to few classes.

Since the present work concerns the properties of transition metals under extreme pres-sures, we will be interested in seeing how stress affects electronic and crystal structure of particular systems. Transition metals mainly attract attention of physicists because they exhibit spontaneous magnetism, so the pressure evolution of their magnetic properties should be studied as well.

In the following paragraphs it will be explained in more detail how structural and mag-netic properties of solids can be studied by means of the DFT calculations.

1.6.1 Structural properties

A problem of finding an atomic configuration corresponding to the local minimum of the total energy is very important in the context of ab initio simulations. These methods can shed light on real physical origins of a certain crystal structure formation and relate it to electronic and magnetic properties of the compound. For example, according to the Stoner model the appearance of spontaneous magnetization tends to decrease system’s equilibrium volume [156]. And first-principles calculations based on the DFT are able to reproduce this physics together with a detailed description of the band structure. However, the so-called structural optimization problem is not always straightforward to solve.

If a periodic system is characterized by one atom per unit cell one can identify few degrees of freedom related with the change of the lattice vectors, i.e. the shape and the volume of a cell. For example, if the symmetry is cubic then the problem becomes easy and has an intuitive solution with the help of the DFT simulations. Namely, one can just vary the lattice constant in order to find the value which corresponds to the energy minimum.

On the other hand, if we consider a system with several atoms per unit cell, the problem becomes much more complicated. The number of degrees of freedom is too high and the “random walk” in these variables is not efficient at all. Instead, thanks to the use of Hellman-Feymann theorem [50], local forces acting on each atom within unit cell can be directly extracted from the calculation. Then the atomic positions can be moved in the direction of the forces (if a used method does not restrict it). After each displacement the density has to be re-calculated to reach self-consistency. In practice few such interactions are enough to find an optimal atomic configuration.

An optimization of geometry of the unit cell requires another quantity as a source of information and is treated differently. For this purpose a quantity called “stress tensor” has to be computed [124–126]. To introduce it, let us consider a general transformation of particles coordinates in a quantum system due to space deformation:

r′_{i,α}= ri,α+
X

β

where i numerates the particles,{α, β} = {x, y, z} are projections on Cartesian axes and εαβ is a so-called “strain tensor”, which in the present context describes deformation of the lattice.

In spirit of the linear response theory, the stress tensor Tαβ is defined as a variation of the total energy with respect to infinitesimal perturbation governed by εαβ:

Tαβ =− ∂Etot

∂εαβ

. (1.22)

Hence Tαβ describes the reaction of the system on certain changes of the lattice. The
trace of T defines internal pressure (i.e. P = 1_{3}P

µ

Tµµ) and shows preferable direction for the change of the volume of the unit cell. Off-diagonal terms are responsible for shear deformations. In general, stress tensor has 9 components, but only 6 are independent due to the space isotropicity. Moreover, the symmetries of the crystal structure relate different components of the tensor. As an example, in the most symmetrical case, i.e. cubic symmetry, the only one independent component remains, i.e. P = Txx. In equilibrium, internal stresses disappear, so all components of Tαβ should vanish. While in order to obtain the structure corresponding to a given external (hydrostatic) pressure Ptarg, one should aim to reach the following relation: Txx = Tyy= Tzz = Ptarg.

In general, the structural optimization has to be done in two steps. A good way of doing it is to start from experimental structure and minimize interatomic forces. Once it is done, the stress tensor can be used to adjust the geometry of the lattice. It is worth emphasizing that the predicted structure depends on the choice of XC potential. If the chosen approximation does not properly describe the GS band structure, there is, in principle, no reason to rely on the results for structural properties (see e.g. [162]).

1.6.2 Magnetism: Mapping on the Heisenberg model

As was already mentioned (2), there are two major models in modern theory of mag-netism: Heisenberg and Stoner ones. In spite of the fact that Stoner mechanism is well reproduced within the DFT [68], this model does not provide an adequate explanation of finite-temperature magnetism. The Curie-Weiss behavior which is reported for nearly any 3d system can not be reproduced: according to the Stoner theory the magnetic moments should disappear above Curie point. Hence it is not surprising that Curie

temperatures (Tc) of transition metals estimated from density of states at Fermi level (DOS(Ef)) are reported to be highly overestimated [69].

Thus, if we want to get a deeper insight into magnetic properties, for instance, to get realistic prediction for Tc or probe the stability of particular magnetic state, it is more useful to use the Heisenberg model for localized spins. Indeed, such approach is not always well-justified when applied to any 3d metal. For example, bulk nickel possessing magnetization of≈ 0.6µB per atom, can be barely considered as a Heisenberg magnet. Indeed, present analysis is supposed to work better for systems like iron and cobalt alloys, which are characterized by significant magnetic moment per ion of the order of few µB.

A phenomenological Heisenberg Hamiltonian in one of its forms can be written as: ˆ

Hexch=− X

i6=j

Jij~ei· ~ej (1.23)

where Jij denotes the exchange integral between magnetic atoms at sites i and j, and ~ei and ~ejare unit vectors in the directions of the local magnetization on sites i and j, respec-tively. The classical5 model treats magnetic moments as vectors of constant magnitude, which interact with each other via parameter Jij. In present notation (Eq. (1.23)), positive J reads ferromagnetic (FM) coupling.

In real magnetic systems Jij’s have several different contributions. A direct exchange given by Eq. (1.6) is only one of them. It can be either FM or antiferromagnetic (AFM), depending on the degree of overlap of two WFs. If we speak about transition metals whose magnetic moments are mainly carried by 3d states, this contribution should decay fast with increase of the distance between spins.

However, there are other exchange mechanisms, like superexchange due to virtual hop-ping from occupied levels of ligands. The sign of this coupling depends on the local geometry and on orbitals involved in the hopping processes [66]. More often superex-change mechanism results in an effective AFM interaction between spins.

5

A quantum version of Eq. (1.23) also exists. According to the basic laws of quantum mechanics, one has to substitute magnetization vectors by corresponding operators.

Conduction electrons are also able to mediate magnetic interactions. Due to their high mobility, Jij(|~r|) can become a rather long-ranged function, having an oscillatory char-acter such that couplings of both signs (FM/AFM) can appear between different pairs. Current mechanism is called Ruderman-Kittel-Kasuya-Yosida (RKKY) [142] interaction and is very common in metallic systems.

Other effective interactions such as “kinetic” or “double” exchange can be also important in the context of 3d metals and their alloys. A book by Fazekas[49] gives a brilliant overview of different exchange mechanisms and explains in detail how they can be derived from many-body Hamiltonians.

Thus Jij is the key quantity of present theoretical method, but in practice has a rather complicated structure with several contributions. Different impacts compete with each other and therefore it is rather difficult to predict even a sign of the total interaction. It was shown by Lichtenstein et al.[105] that there is a way to extract J parameters from the GS DFT calculation.

The primary idea of the suggested approach is to consider an infinitesimal rotation of the spin i on angle θ and then write second variation of the total energy with respect to this perturbation. Starting from the FM state from Eq. (1.23) one obtains:

ˆ

H =_{−}X

i6=j

Jij|~ei| · |~ej| cos θ ≈ − X i6=j Jij+ X i6=j Jij θ2 2 . (1.24)

Then the same procedure has to be performed on a real spin-polarized Hamiltonian,
which comes from converged DFT calculation. Projected on atomic states Hamiltonian
can be expressed in the matrix form as ˆH_{ijmm}σσ′ ′ =< im′σ′| ˆH|imσ > where i denotes
site, m is magnetic quantum number and σ = _{{↑, ↓} is electron spin projection. It is}
also useful to formally define the corresponding Green’s function as ˆG(z) = (z− ˆH)−1.
Such quantities are more easily accessed within LMTO formalism which is the most
widely-used approach for such type of studies.

In terms of electronic Hamiltonian the above-mentioned transformation corresponds to an application of the following operator:

ˆ U = exp i~θ·S~ˆ ≈ 1 + i~θ ·S~ˆ−1 2(~θ· ˆ ~ S)2, (1.25)

whereS =~ˆ ~σˆ_{2} and ˆ~σ ={ˆσx, ˆσy, ˆσz} is a vector of Pauli matrices.

Using “local force theorem“ [129], which states that variation of the total energy with
respect to to some perturbation (δE) is a sum of changes in one-electron energies, it
can be shown that for small values of θ there is an exact mapping of real electronic
Hamiltonian on the Heisenberg one. So one obtains the same form of variation as given
by Eq. (1.24), where intersite exchange Jij is expressed in terms of band structure
quantities:
Jij = 1
4πℑ
Z Ef
−∞
Tr{m}(∆iG↑_{ij}∆jG↓_{ji})dz. (1.26)

Here ∆i = ( ˆHii↑ − ˆHii↓) is an exchange potential on the i-th site and Gσij is a matrix of intersite Green’s function, which describes propagation of an electron with spin σ from site i to j. Here z is a complex energy variable of the form E + iǫ. Integration has to be performed over z, in order to avoid poles of the Green’s function.

Suggested approach allows to compute exchange integrals between any pair of spins in
a real magnetic system, assuming that the DFT provides a correct description of its
electronic structure. This approach was applied to series of transition metal alloys and
provided nice estimations of Tc as compared with experimental data [56, 74, 130]. In
practice it turns out that the agreement is better for compounds with larger values of
magnetization. This is understandable, since the squared magnitude of a quantum spin
S is _{|S|}2 _{= S(S + 1), while in classical Heisenberg model it equals S}2_{. Both these}
expression coincide in the case of infinitely large spin S, meaning that the larger the
spin value the closer its behavior to the classical one. This gives an idea about the range
of application of Lichtenstein’s approach.

It has to be emphasized that calculated J-parameters are extracted from the GS with a certain (assumed) magnetic order. Therefore these parameters are not universal quanti-ties and in principle there is no guarantee that extracted from different reference states values will coincide.

However this information can be useful for studying the stability of a particular magnetic state. For this purpose obtained J’s can be used to find low-energy magnetic excitation (i.e. frozen magnon) spectra [130].

**q**
**z**

Figure 1.2: _{Schematic representation of a frozen magnon. Arrows show the direction}
of local magnetization, which is initially aligned along Z axis.

1.6.2.1 Frozen magnons simulations

Magnons or spin waves (SWs)6 are quasiparticles representing a certain type of excita-tions in the spin density. They can be seen as infinitesimal deviation of one spin’s orien-tation which then propagates through the entire periodic system with a given wavevector ~q. Real SWs are observed in inelastic neutron scattering (INS) experiments and provide information about system’s dynamical magnetic susceptibility χ(ω, ~q).

In the framework of “frozen magnons” there is no real motion. Imagine that we take a snapshot of a SW at a certain time – it will look like a spin spiral with small transverse components, as shown on Fig. 1.2.

This is a valid representation of real magnons in adiabatic limit, i.e. when spin dynamics is defined on a much shorter time-lengths than changes in the electronic potential energy. Indeed, one of the possibilities to model SWs is to directly calculate the total energy of such spin spirals. This can be done with the help of generalized Bloch theorem [146]. We will follow another strategy and use extracted Jij parameters. For this purpose we consider a simple gyroscopic equation of motion which governs SW dynamics:

d ~Sj dt =− 1 ~ ~ Bj× ~Sj , (1.27)

where ~Sj =|Sj|~ejis a vector of the magnetic moment located at the position ~Rj; ~Bjis an effective field acting on the corresponding spin, which appears from the spin Hamiltonian : ~ Bj =−∂ ˆH ∂ ~Sj . (1.28) 6

This term must be distinguished from the spin density waves (SDW), which are related to the modulation of the spin density. SDW does not imply systems’s excitation.

In the simplest case of FM system containing one magnetic atom per unit cell and described by Heisenberg Hamiltonian (Eq. (1.23)) it is easy to show that energies of spin waves propagating with wavevector ~q are given by:

E(~q) = 4µB
|S|
X
j6=0
J0j
1_{− exp (i~q · ~}Rj)
(1.29)

Eq. (A.1) can be generalized for the case of several magnetic sublattices and different their arbitrary orientations. A detailed derivation of the corresponding formulas is given in the AppendixA. In these cases one has to deal with a linear system of coupled equa-tions, which solution will give few branches of spin waves. One of them will necessarily possess the following property: lim

q→0E(q) = 0. This is a so-called “Goldstone” mode which is responsible for low-energy excitations, we will be interested in. Appearance of negative/imaginary eigenmodes in this mode will indicate instability of the assumed magnetic order.

In this thesis the calculation of SWs Goldstone mode will be performed for certain
magnetic alloys. Note that higher-lying (”optic“) modes will not always be shown in
present work since it is out of the scope of the study. In reality, these branches will
be considerably attenuated due to presence of another type of spin excitations called
”Stoner excitations“. They appear when majority-spin electron jumps to unoccupied
spin-down state. This process requires to flip the spin and, therefore, costs some finite
energy of the order of intra-atomic exchange _{∼ 1 eV.}

### 1.7

### Conclusions

In this chapter we have introduced the standard methods, which are used for first-principles modeling of the electronic structure in solids. It has to be emphasized that the DFT is an exact theory. Yet, its realizations should be called ”ab initio“ with certain provisos. Within this theory, there is a choice of the XC potential which implies some approximations. For many systems these approximations are acceptable and the method can be used to investigave microscopic mechanisms, which define the overall system’s behavior.

It is a powerful and widely used tool in nowadays condensed matter physics. In the next chapters we shall see how the present theory can be applied to study magnetic and structural properties of various 3d metal-based systems.

## K-edge XMCD study of transition

## metals under high pressure

### 2.1

### Introduction: experimental technique

It was Faraday who first pointed out peculiarities in the interaction between a light and magnetized matter [48]. He discovered that if a sample is exposed to a magnetic field, shining a linearly polarized light in the direction of the field on it causes rotation of the corresponding polarization vector. Later Kerr found the same phenomenon for a reflected light, which permitted to the observe domain structure in ferromagnetic compounds (see e.g.[169]). These findings opened a new branch of effects called “magneto-optical” and since then their number increased dramatically. Nowadays they are one of the primary tools to study magnetic materials.

Magneto-optical experiments were initially carried out using solely the visible light. However, the same phenomena take place for other parts of the spectrum of electromag-neti radiation. And the biggest achievements in this field are related with the use of x-ray photon energies.

The main merit of x-rays is the element-selectivity. A simple estimates for hydrogen-like atom show that energy of 1s level of an element with atomic charge Z should be

proportional to Z2 [16]. Therefore, absorption edges1 of all atomic species are
well-separated in the absolute energy scale. Corresponding energies for the majority of
elements from periodic table fall into the range, which is covered by soft and hard x-ray
regimes2_{. Thus exposing a sample to the x-ray beam of a certain wavelength permits to}
investigate the states of this particular element and not the others.

In terms of absorption of electromagnetic waves, there is an interesting magneto-optical effect: magnetic samples absorb the light with right and left circular polarization (RCP and LCP) differently. The effect is called Magnetic Circular Dichroism (MCD). Its man-ifestation in x-ray regime (XMCD) was predicted theoretically by Erskine and Stern [47] for M2,3-edges of Ni. However, the first experimental confirmation of the XMCD effect was obtained more than ten years later by van der Laan et al. [164].

It can be shown that the change of incident light helicity is equal to the invertion of magnetic field direction, since both operations have a meaning of the time inversion. So the XMCD signal is defined by taking the difference between X-ray absorption spectra measured with parallel and antiparallel (µ+ and µ−, respectively) orientations of the magnetization with respect to beam helicity:

µXM CD(ω) = µ+(ω)− µ−(ω). (2.1)

The pioneering experimental study of the XMCD in transition metals was performed by Sch¨utz et al. [149] at the K-edge of iron. However, the biggest challenge was to address L2,3-edges, since the final state of this process is in 3d shell, where main magnetic properties come from. Chen et al. [29] were the first who succeeded in carrying out such experiment on pure nickel. Since few years after this work the XMCD has already become one of the most widely-used tools to probe orbital magnetism [139]. Using this technique one is able to resolve different contributions to spin and orbital magnetizations originating from inequivalent atomic species (see e.g. Ref. [38]).

1

This is the energy which is needed to move an electron from corresponding bound state to the continuum. Notations K, L1, L3,2mean that 1s, 2s, 2p electron levels are, respectively, involved.

2

Soft x-rays are usually called the ones whose energies are in the region between 0.1 and 1 keV, e.g. L2,3-edges of 3d metals. Hard x-rays regime is in between 1 and 10 keV, e.g. K-edges of the same class